THE COMPOUNDING OF SHORT FIBRE

REINFORCED THERMOPLASTIC COMPOSITES

A thesis submitted for the degree of Doctor of Philosophy

by

Paul David Shipton

Department of Materials Technology, Brunel University

July 1988

### BEST COPY

### AVAILABLE

### Variable print quality

Brunel University

Department of Materials Technology Uxbridge, Middlesex, UB8 3PH

Paul David Shipton

The Compounding of Short Fibre Reinforced Thermoplastic Composites Ph. D. Degree

1988

ABSTRACT

It is generally accepted that the mechanical properties of short fibre

reinforced thermoplastics do not correspond with the high mechanical properties of fibres used to reinforce them.

A study is made into the methods of compounding reinforcing fibres into thermoplastics to produce short fibre reinforced thermoplastics of enhanced

properties.

The initial method chosen for investigation is the twin screw extrusion

compounding process. Variables such as fibre feeding arrangement and extrusion screw design are found to be factors influencing the properties of carbon and glass reinforced nylon 6,6. Use is made of computer programs to predict

properties, assess compound quality and estimate fibre-matrix bond strength.

Investigations indicate that the presence of reinforcing fibres with enhanced lengths does not result in the predicted property increases. The

reasons for this shortfall are believed to lie in unfavourable fibre orientation in injection mouldings and the reduced strain to break of these materials.

Short Kevlar reinforced thermoplastics are compounded and their mechanical properties assessed. The reasons for the poor mechanical properties for these materials are identified as a poor bond strength between fibre and matrix,

the formation of points of weakness within the fibres by the compounding and moulding processes and the coiled arrangement of fibres present in injection

mouldings.

A method suitable for the routine assessment of fibre-matrix bond strength is used to examine combinations of fibre and thermoplastic matrix. A comparison is made of the values derived from this method with values calculated from

stress-strain curves of injection mouldings. This allows an understanding of the nature of the fibre-matrix bond yielded by compounding and injection moulding steps.

A description is given of a novel method designed to overcome the

limitations of conventional compounding routes to produce long fibre reinforced injection moulding feedstock. Further work is necessary before this method

is a feasible production technique.

Abstract

It is generally accepted that the mechanical properties of short fibre reinforced thermoplas- tics do not correspond with the high mechanical properties of fibres used to reinforce them.

A study is made into the methods of compounding reinforcing fibres into thermoplastics to produce short fibre reinforced thermoplastics of enhanced properties.

The initial method chosen for investigation is the twin screw extrusion compounding pro- cess. Variables such as fibre feeding arrangement and extrusion screw design are found to be fac- tors influencing the properties of carbon and glass reinforced nylon 6,6. Use is made of computer programs to predict properties, assess compound quality and estimate fibre-matrix bond strength.

Investigations indicate that the presence of reinforcing fibres with enhanced lengths does not result in the predicted property increases. The reasons for this shortfall are believed to lie in unfavourable fibre orientation in injection mouldings and the reduced strain to break of these materials.

Short Kevlar reinforced thermoplastics are compounded and their mechanical properties assessed. The reasons for the poor mechanical properties for these materials are identified as a poor bond strength between fibre and matrix, the formation of points of weakness within the

fibres by the compounding and moulding processes and the coiled arrangement of fibres present in injection mouldings.

A method suitable for the routine assessment of fibre-matrix bond strength is used to exam- ine combinations of fibre and thermoplastic matrix. A comparison is made of the values derived from this method with values calculated from stress-strain curves of injection mouldings. This allows an understanding of the nature of the fibre-matrix bond yielded by compounding and injection moulding steps.

A description is given of a novel method designed to overcome the limitations of conven- tional compounding routes to produce long fibre reinforced injection moulding feedstock. Further work is necessary before this method is a feasible production technique.

Wer Immer Strebend sich bemuht, den Kornen Wir erlosen

Whosoever unceasingly strives upward...

him can we save.

GOETHE

The Compounding of Short Fibre Reinforced Thermoplastic Composites

Page No.

Abstract

Chapter 1 General Introduction

1.1 The Problems Associated With The Incorporation of Short Fibres into Thermoplastics

1.2 Review of Adopted Approach to Produce High

Performance Short Fibre Reinforced Thermoplastics 1.3 Outline of Thesis Structure

1.4 Aims and Objectives 1.5 Reinforcement Theory

1.5.1 The Stiffness and Strength of Continuous Fibre Composites

1.5.2 The Stiffness and Strength of Short Fibre Reinforced Thermoplastics

1.5.3 The Stiffness and Strength of Partially Aligned Composites

1.5.4 The Toughness of Discontinuous Fibre Composites

Chapter 2 Review of Literature

I

2 3 4 4

5

6

11

14

2.1 Composite Materials 17

2.2 Reinforcing Fibres 18

2.2.1 Carbon Fibres 19

2.2.3 Glass Fibres 20

2.2.4 Kevlar Fibres 2.3 Compounding 2.3.1 Introduction

2.3.2 Melt Compounding Other Than Extrusion 2.3.3 Extrusion Melt Compounding

2.3.4 Injection Moulding

2.3.5 Conclusions from Reviewed Literature 2.3.6 Twin Screw Extrusion

2.3.6.1 Twin Screw Extruder Processing

2.3.6.2 Characteristics of Twin Screw Extruders

2.4 The Compounding of Kevlar Fibre into Thermoplastics

2.5 Methods to Evaluate the Effect of Compounding Technology on the Stress Transfer Interface of Short Fibre Reinforced

Thermoplastics

Chapter 3 Experimental

3.1 Materials

3.1.1 Matrix Systems

3.1.2 Precompounded Materials 3.1.3 Reinforcing Fibres

3.2 Compounding Extruders

3.2.1 Gays TS40-DV-L Twin Screw Extruder

3.2.2 Baker Perkins MPC/V50 Compounding System 3.2.3 Reinfenhauser Single Screw Extruder

3.3 Injection Moulding 3.4 Fibre Extraction

3.4.1 Extraction of Carbon Fibres From Nylon 6,6

21

22

25

26 27

29 29 31 33 36

36

39 39 40

40 41 42 42 43 43

3.4.2 Extraction of Glass From Nylon 6,6 or Polypropylene 43 3.4.3 Extraction of Kevlar fibres from Polypropylene 44

3.5 Fibre Length Determinations 44

3.6 Mechanical Testing

3.6.1 Tensile Properties 46

3.6.2 Flexural Properties 46

3.6.3 Impact Properties 47

3.7 Scanning Electron Microscopy 49

3.8 Prediction of Composite Properties and Assessment

of Compounding Techniques 50

3.9 Investigations of Transcrystallinity 50

3.10 Experiments Performed Compounding Carbon and Glass (Brittle Fibres) into Thermoplastics

3.10.1 Introduction 51

3.10.2 Experiments Based on the Gay's TS40-DV-L Twin Screw

Extruder 51

3.10.3 Experiments Based on the Baker Perkins MPC/V50

Compounding System 52

3.11 Experiments Performed Compounding With A Ductile Fibre, Kevlar 49

3.11.1 Introduction 53

3.11.2 Investigations Based on the Reifenhauser Single

Screw Extruder 53

3.11.3 Investigations Based on the Baker Perkins MPC/V50

Compounds 54

Chapter 4 Results

4.1 Experiments Performed Compounding Brittle Fibres in the Gay's TS40-DV-L Twin Screw Extruder

4.1.1 Experiment BRITTLE 1 56

4.1.2 Experiment BRITTLE 2 56

4.1.3 Experiment BRITTLE 3 57

4.1.4 Discussion 58

4.2 Experiments Performed Compounding Brittle Fibres in the Baker Perkins Compounding System

4.2.1 Experiment BRITTLE 4 61

4.2.2 Experiment BRITTLE 5 65

4.2.3 Experiment BRITTLE 5 66

4.2.4 Discussion 67

4.3 Experiments Performed Compounding Kevlar Fibres in the Reinfenhauser Single Screw Extruder

4.3.1 Experiment KEVLAR 1 76

4.3.2 Experiment KEVLAR 2 78

4.3.3 Discussion 78

4.4 Experiments Performed Compounding Kevlar Fibres

in the Baker Perkins Compounding System

4.4.1 Experiment KEVLAR 3 81

4.4.2 Experiment KEVLAR 4 82

4.4.4 Discussion 83

4.5 Impact Properties of Short Fibre Reinforced Thermoplastics

4.5.1 Impact Properties of Kevlar Reinforced

Thermoplastics 89

4.5.2 The Estimation and Prediction of Fracture Energy for Glass Reinforced Nylon 6,6

4.5.3 Discussion 92

Chapter 5 The Determination of Critical Fibre Length in Short Fibre Reinforced Thermoplastics

5.1 Introduction 98

5.2 Experimental 98

5.3 Results 101

5.4 Discussion 102

Chapter 6 The Production of Fibre Reinforced Thermoplastics Using an Especially Designed Crosshead die

6.1 Introduction 105

6.2 Experimental 107

6.3 Results 108

6.4 Discussion 110

6.5 The Injection Moulding and Mechanical Properties

of a "Long Fibre" Glass Reinforced Nylon 6,6

Material (ICI Verton) 111

Chapter 7 Conclusions and Suggestions for Further Work

7.1 Conclusions 113

7.2 Suggestions for Further Work 115

Acknowledgements References

Appendix

1.1 The Problems Associated with the Incorporation of Short Fibres Into Thermoplastics

Thermoplastics containing short fibres were first introduced with the intention of offering a

new range of materials with intermediate properties between high tonnage commodity plastics and the sophisticated continuous fibre composites well established in the aerospace industry. The increase in stiffness and strength compared with the parent thermoplastic was modest but sufficient to establish the class of material in lightly stressed applications.

Short fibre reinforced thermoplastics are now well established engineering materials and are now used to fabricate many articles traditionally produced from metals.

The production of components is normally carried out in two stages; compounding of the polymer followed by injection moulding. Direct attempts to injection mould fibre/polymer blends can lead to problems of poor surface finish, high differential shrinkage and variable strength due to the presence of undispersed bundles in the finished article.

It has become apparent that the detailed procedures used for compounding have a marked effect on the properties of the moulded component, and work has been directed towards a more fundamental understanding and subsequent control of the factors which determine the desired properties.

The major variables for influencing the performance of short fibre reinforced thermoplastics are the adhesion between fibre and matrix, the length of the fibres and fibre orientation.

Care is required in the compounding operation to produce an adequate dispersion of bundles while preventing significant fibre attrition.

The selection of the appropriate compounding technology is consequently dependent on the requirements of fibre length and degree of dispersion of the fibres throughout the matrix. The most common method of compounding involves the use of a single or twin-screw extruder to mix chopped fibres and matrix and produce an extrudate which can be subsequently pelletized to give feedstock for injection moulding.

This research is centred on the development of compounding extrusion techniques that

-2-

allow more effective utilization of the properties of high performance reinforcing fibres. This area of investigation is vital if the mechanical properties of fibre reinforced thermoplastics are to be enhanced compared with currently available products.

1.2 Review of Adopted Approach to Produce High Performance Short Fibre Reinforced Thermoplastics

Three basic approaches were used in this study to produce high performance short fibre reinforced thermoplastics. The first approach was to compound inherently brittle glass and car- bon fibres into thermoplastics in such a way that fibre length was retained. After considering the available literature, the starting point for this approach was the use of a twin screw extruder where fibres could be added to a premelted matrix. The first three experiments, based on a small laboratory twin screw extruder, determined the most important factors that influenced the fibre length distribution of short brittle fibre reinforced thermoplastics. The three subsequent series of experiments, which were performed on a full scale production twin screw compounding system, utilized the knowledge gained in the initial three experiments. A wide range of compounding arrangements were investigated and detailed characterisation procedures were carried out on the materials produced. An optimum screw configuration for producing carbon fibre reinforced nylon 6,6 was derived.

The second approach adopted was to compound Kevlar 49, an inherently tough fibre into thermoplastics. Although Kevlar 49 is flexible and abrasion resistant, its tensile properties rank close to carbon and glass. Because of its non brittle properties, it was thought that this fibre could be incorporated into a thermoplastic with a substantial proportion of its fibre length retained. As little work had been previously carried out on the incorporation of Kevlar into thermoplastics, the starting point for this approach was single screw compounding. The limitations however in sin- gle screw compounding were quickly realised. Successful compounding was eventually achieved using the production scale twin-screw compounding system.

The third approach adopted was to employ a novel technique in which the limitations which became evident in the first two approaches would be overcome. The technique adopted was a

-3-

specially designed crosshead die.

13 Outline of Thesis Structure

This chapter includes a brief review of composite theory relevant to this study. The litera- ture survey, Chapter 2, starts with a concise discussion of the nature of composite materials and endeavours to outline the characteristics of the reinforcing fibres used in this study. An attempt is made to review critically the current understanding of the compounding of short fibres into ther- moplastics. In the survey, conclusions are made and literature concerning a selected technique, twin screw extrusion is presented. The literature survey concludes with an examination of the computational methods that have been used to assess the effectiveness of compounding tech- niques.

Chapter 3 firstly reviews the materials used in this thesis, describes the machines used for compounding and the conditions used for the moulding of the materials. The techniques employed to assess the materials are detailed, these include fibre length properties, mechanical testing, scanning electron microscopy and the analysis and prediction of material properties by computer programmes. The final part of Chapter 3 describes in detail the compounding experi- ments performed.

Chapter 4 presents firstly the experimental results for the preliminary investigations based on a small scale laboratory twin-screw extruder. In the following section the results are dis- cussed. Results are then presented for compounding glass and carbon fibre into nylon 66 on a production scale twin-screw compounder of greater power and output, these results are then dis-

cussed. The second part of Chapter 4 is based on the results and subsequent discussion of Kevlar reinforced thermoplastics. A single screw extruder and a twin-screw compounder were used to incorporate Kevlar fibres into thermoplastic matrices.

From a practical point of view composite materials in addition to being stiff and strong must also be reasonably resistant to impact loading. The final part of Chapter 4 presents and discusses the impact properties of some of the materials produced in the compounding experi-

-4-

ments. The impact properties of short fibre Kevlar reinforced thermoplastics were measured in an attempt to rank them against conventional glass reinforced thermoplastics. For selected glass reinforced nylon 6,6 compounds the contribution to fracture energy Gc by fibre pull-out was estimated and compared with measured values.

Chapter 5 describes the techniques used for the determination of critical length of fibres in short fibre reinforced thermoplastics. The chapter is divided into four sections to describe fully the technique and present the results.

Chapter 6 presents a description of a novel technique developed for the production of fibre reinforced thermoplastics using a specially designed crosshead die.

The concluding chapter, Chapter 7, seeks to draw together the findings gathered throughout the study and make recommendations for future investigations.

1.4 Aims and Objectives

(i) Using selected types of compounding machinery, to investigate the limitations of com- pounding brittle types of fibre such as glass and carbon into thermoplastics and suggest compounding arrangements that may be used to produce mouldings with enhanced proper- ties.

(ii) To investigate methods of compounding Kevlar 49, a tough fibre with good mechanical pro-

perties, into thermoplastics and examine the salient properties of the resulting composites.

(iii) To examine the properties of the bond between selected thermoplastics and reinforcing fibres and develop methods for assessing the effectiveness of the bond.

(iv) On the basis of the findings made, to develop an alternative compounding operation which would overcome any difficulties found with conventional techniques.

1S Reinforcement Theory

The prediction of the mechanical properties of a fully aligned long fibre reinforced compo- site is a difficult mathematical problem, particularly when the load is not applied along the fibre

-5-

axis. To perform the same exercise in a short fibre reinforced composite is even more difficult.

The fibres can not be regarded as infinitely long and in addition a real moulded component exhi- bits a very complex fibre orientation distribution. Any realistic reinforcement theory has to include the effect of fibre length distribution and a distribution of fibre orientations with respect to the applied load. While the stiffness of short fibre reinforced thermoplastics has received the most attention and can be predicted fairly accurately, properties such as strength and toughness are difficult to predict even for continuous fibre composites. The corresponding problem with short fibre reinforced thermoplastics has not received much attention.

1.5.1 The Stiffness and Strength of Continuous Fibre Composites

The simplest type of fibrous composite is one with straight parallel isotropic and homogene- ous fibres in a isotropic homogeneous matrix. Here the mechanical properties of the composite can be explained simply in terms of the mechanical properties of fibre and matrixl. When a load is applied parallel to the fibres, effectively little load is carried by the matrix. The principal pur- pose of the matrix is to bind the fibres together. For long fibres, stress is constant over the whole length of the fibres. This idealised composite is the starting point for all theories of reinforce- ment. When a load is applied parallel to the fibres, the load is distributed in proportion to the relative volume fractions of the fibre and matrix, the composite's mechanical properties in this direction can be described by The Rule of Mixtures. If we assume the fibres and matrix behave elastically and are perfectly bonded to each other and consider what happens when a strain c is applied uniformly in the fibre direction (Figure 1), the total force will be the sum of the forces in the fibre and matrix.

The Young's modulus of the composite Ec in the fibre direction is: - Ec=VfEt+(1-Vf)E,

where

Vf = volume fraction of fibres Ef = Young's Modulus of fibres F,, = Young's Modulus of matrix

(1)

-6-

The tensile strength of the composite a, is given by: -

au=aufVCFc'm(l-Vi) (2)

where

c;, ,f= ultimate strength of fibre

a`m = stress in matrix at the ultimate strain of the fibres

Whereas equation 1 only holds true for stiffness with their components in the elastic state equation 2 may still be used with the matrix in the plastic state. However in practice the strength of a continuous fibre reinforced composite rarely approaches the value given by the equation.

Whereas stiffness can be predicted for such a system fairly accurately by the rule of mixtures, strength is a difficult quantity to predict using the eile of mixtures even for such an idealised sys- tem.

1.5.2 The Stiffness and Strength of Short Fibre Reinforced Thermoplastics

In the case of discontinous fibre composites the only continuous phase is the matrix phase so the load is transferred to the stiff fibre via shear stresses at the interface.

For the purpose of this survey, a short fibre reinforced material is one in which the fibres have an aspect ratio (length: diameter) of between 10 and 1000(2). To consider the stiffness and strength of a discontinuous fibre composite we need to take into account how stress is transferred to or from the fibre.

Five theories3 have been presented on the longitudinal stress distribution along the fibre matrix interface. Four of these have considered both the fibre and matrix in the elastic state the fifth has considered the matrix in a plastic state. These are reviewed briefly in Figure 2a and b.

Composite materials are commonly used in the range of stresses between the very low stresses at which the Cox theory can be used, and the failure stresses described by the failure theories. The incompatibility of the assumptions needed for the modulus expression and those needed for the strength expression received attention by Piggot9. Piggot extended earlier theories of reinforcement and estimated the effect on the stress-strain curve of factors such as friction

-7-

between fibre and matrix, residual and shrinkage stresses. Unfortunately little data exists on these parameters so there is little empirical evidence to substantiate his theory.

In this thesis it was decided to use the Cox analysis to predict tensile stiffness, as at low lev- els of strain where tensile stiffness is meaured, the thermoplastic matrix at the interface between the fibre and matrix could be expected to behave elastically and not yield or debond from the fibre. The Kelly-Tyson analysis was used to predict properties such as interfacial shear strength and ultimate tensile strength at higher values of strain where the matrix was likely to have yielded and plastic deformation could take place at points along the interface.

Each of the chosen analyses will now be discussed in more depth.

The Cox Shear Analysis The main assumptions made by Cox are: -

(i) A round fibre is surrounded by a cylindrical matrix as shown in Figure 3.

(ii) The transfer of load from the matrix to the fibre depends on the difference between the actual displacement of a point on the interface and displacement than would exist if the fibre were absent.

(iii) A perfect bond exists between fibre and matrix.

(iv) There is no load transfer through the ends of the fibre.

With reference to Figure 3 consider a fibre of length 1 and radius r embedded in a matrix.

We assume that the matrix as a whole is strained homogeneously by the application of a load applied parallel to the fibre axis. Since the shear stress ti at the fibre-matrix interface will vary along the fibre, so also will the tensile stress in the fibre. Considering a small element of the fibre length Sx, the net tensile load SF across this element must be balanced by the shear force at the interface i. e.

8F=ti2nr8x or

d -411=2ir (3)

when Sx- 40

-8-

Since the assumption has been made that the matrix and fibres are strained elastically, then c oc y where y is the shear strain developed at the fibre-matrix interface. Furthermore, y can reasonably be expected to be proportional to the difference in elastic displacement u in the fibre at some point x from one end and the elastic displacement v of the matrix at the same point, if the fibre were absent. Hence we may write: -

dR

-H(u-v) (4)

where H is a constant for a particular composite.

From Hooke's Law

F EfAf

dx (5)

where Ef = Young's modulus of the fibre Af = Area of cross-section of a fibre Differentiating equation (4) with respect to x we have: -

d2F

_H

du _

dv dx2 dx dx

but dx Af from equation (5), while = c, the strain in the matrix.

hence dF z

_H F

dx2 EfAe

This second order differential equation has a solution of the form: - F= EfAf c+B sinhßx + Ccosh ßx

where ß=Äf and B and C are constants of integration, whose values are determined by two boundary conditions. These are that no loads are transferred across the end faces of a fibre i. e. F=0 at x=0 and x =1. We then obtain for the distribution of tensile stress along the fibre: -

F cosh (112-x)

a Af =E fe 1-

coshßll2

From this result, the average tensile stress developed in the fibre can be easily evaluated and is given by: -

-9-

Qf= Ef c I- tann l/Z ß1R

The average longitudinal stress in a composite containing a volume fraction of fibres Vf can then be calculated as a weighted average of the stresses developed separately in the fibre and matrix i. e.: -

aC = Vf 6f+ (1-Vf)Qm

where am is the stress developed in the matrix.

since Qm=Eme, where Em = Young's modulus of the matrix

aý=VfEf 1- Rll/2 ]+(1_Vf)EnE The effective longitudinal modulus of the composite is given by: -

Ec_ Ec

_VIEI I-tR ril

+(I-Vf)Em (6)

If the mean centre-to-centre separation of the fibres normal to their length is R then Cox showed that: -

2nGm H=

loge

Ir

If it is assumed the fibres are arranged hexagonally the volume fraction of fibres: - 22r2

Vf =

IR2

The largest value of interfacial shear stress occurs at the ends and is zero in the middle. The main source of error in the analysis is the manner in which the shear stress is assumed to decay around individual fibres. The Cox analysis ignores interactions between adjacent fibres. Using finite ele- ment analysis, Chen10 showed that due to the discontinuity of neighbouring fibres in discontinu- ous fibre composites, the portion of fibre adjacent to a neighbouring fibre end must be under greater stress than it would be in the continuous case. This concept was denoted the perturbation effect and cannot be predicted by the Cox shear lag analysis. Tyson and Davis11 showed using a

-10-

two dimensional photoelastic model the existence of high shear stresses near fibre ends, which peak to values greater than these predicted by shear lag theory. The existence of these high stresses at fibre ends was also confirmed by Chen and Lavengood12 by a finite element analysis.

The artificial model of fibre packing in the Cox model also becomes more difficult when extended to non aligned fibres.

Figures 4 to 7 show the dependence of predicted stiffness on average fibre length for the four types of composite material produced in this thesis.

The Kelly Tyson Analysis

Whenever a thermoplastic is loaded in tension, if the applied load exceeds a certain value the material shows a yield point. When a thermoplastic is used as a matrix material for a short fibre reinforced thermoplastics the shear stresses developed towards the end of the fibres can exceed the shear strength of the matrix t.. The effect is to limit the maximum shear strength at the fibre interface to T,,. Whereas in the Cox analysis the variation of tensile stress towards the fibre ends is strictly non linear, the presence of a constant shear strength rm will lead to a simple linear increase in tensile stress from the ends of the fibre until a constant tensile stress of Ef e is reached. In composites containing very short fibres the shear stress induced at the fibre-matrix interface will cause failure at the interface before the maximum stress in the fibre reaches the fibre failure stress, while in composites containing longer fibres the fibre failure stress will be reached first and failure will occur by fibre breakage. There thus exists a 'critical fibre length' (la where the fibre failure stress and shear failure stress are reached simultaneously. It can be shown that this is given by

jc _ 2ý where

o ,, f fibre strength d fibre diameter

(7)

, ru interfacial shear strength

-11-

The variation of tensile stress with fibre length according to this analysis is shown in Figure 8 for a fibre (a) less than (b) equal to and (c) greater than the critical length

If ßf is the average stress carried by the fibre

äf= 1- 2. l af for We

l

ac =GUM 1- 2+ (1- Vf)a`m

where a`m = stress in the matrix at the ultimate strain of the fibres. However if the fibres are

shorter than 1, the maximum fibre stress is only 2j1/d and the mean strength will be half of this.

The composite strength will be

ßuc= Vf+(I-Vf)O'm

On the basis of this theory even if the ratio of j

is as low as 10 then 95% of the strength Ic

obtained with continuous fibres can be obtained with aligned discontinuous fibres13

In all the short fibre reinforced thermoplastics considered in this study, however, there are distributions of fibre lengths. Then it is necessary to sum the contributions arising from the fibres of sub critical and super critical length to give an equation of the form advocated by Nielson and Chen 14. For aligned fibres: -

Tvlivfi Q"c= ý,,

d +ý, ßtVf _-Lc i +(1-Vf)ß`m (8)

As was the case of the Cox shear lag analysis, the main error inherent in the Kelly-Tyson analysis is the neglection of fibre-fibre interaction In a study directed at predicting the tensile strength of discontinuous aligned composites, Riley-' lconcluded that due to the concentration of stress that occurs at a fibre end which must be taken up by surrounding fibres, discontinuous com- posites will never achieve strengths greater than 6/7 of the continuous fibre strength.

-12-

15.3 The Stiffness and Strength of Partially Aligned Composites

The description of the theory so far has been concerned with the mechanical properties of uniaxially aligned short fibre composites. In moulded composites however, fibres are seldom aligned, so some provision must be made in the theoretical analyses to allow for partially orien- tated systems.

The prediction of stiffness of partially orientated composites has been approached by a number of investigators. Krenchel16 and Cox4 evaluated the relative efficiency of fibres in each orientation followed by an averaging procedure for the whole composite. In his approach, Kren- chel adopted an orientation efficiency factor of reinforcement too to allow for reduction of rein- forcement of fibres lying at an angle 0 to the stress axis. In the general case of transverse isotropy Krenchel proposed that ilo could the form

rio =E an Cos4 On

n

where Fa, =1. an is the volume fraction of fibres lying at an angle On to the stress axis and n is the

n

number of angular intervals into which the fibre orientation is divided.

Since in the case of this study we are concerned with short fibres the total efficiency factor where 1- tanh 12

i1= iloil I X11=

ß[2 if the Cox analysis is used.

The total stiffness of the composite is then given by: -

Ec=11o 1iVfEf +(1-Vf)Em

Jerina et a117 predicted stiffness by treating the composite as an assembly of plies. The stiffness of each layer is predicted or measured experimentally and the stiffness of the plies are summed to give the stiffness of the composite, this method is reported to be comparatively

straight forward to apply.

In the prediction of stiffness by Brody and Wardle, the composite is regarded as an aggre-

gate of sub-units, each sub-unit possessing the elastic properties of a reinforced composite in

13-

which fibres are continuous and fully aligned. Involved algebra is required to obtain upper and lower bounds for composite elastic constants.

As in the case with stiffness, the strength of an aligned short fibre composite decreases as the angle between the fibre axis and loading direction increases. The prediction of strength anis- tropy requires a failure criterion. There are two criterion that have received wide spread attention.

Stowell and Liu19 invoke a maximum stress criterion and define three failure mechanisms. For stresses directed along or at small angles 0 to the fibre axis, failure will be controlled by fibre strength. At larger angles the dominant failure made will be due to shear processes. At very large 0, approaching 90° the mode will change again to one of transverse failure either in the matrix or at the interface.

These may be expressed mathematically as follows: -

aO=a,. Sec2 0

for fibre tensile failure

aO = 2ti, cosec2O for shear failure parallel to the fibres

a9 = a, Icosec2O for tensile failure normal to the fibres

ßu9 is the composite strength at an angle 0 to the fibres, Qc and a,,, are the strengths of the uniax- ially aligned composite with and normal to the fibres, and Tc is the in-plane composite shear strength. An alternative failure criterion found to fit strength data for short fibre composites is due to Hill20 and Azzi and Tsai21. They used a maximum distortional energy based on the Von Mises criterion.

The approach adopted by Krenchel for predicting stiffness can also be applied to obtain an estimate of the strength of a composite containing misaligned fibres. Lees22 integrated the Stowell-Liu equations over all angles for the special case where the fibres were random in plane

14-

to give the following equations for the average strength of the composite

,

7c

<a >= 2c 2+ 104 Qucaut tuc

as before ; c is the composite shear strength and (T. is the transverse strength of the uniaxially aligned composite.

Using a similar approach to Lees, Chen23 suggests that the predictive equation should be

<a ,>=

2'ß'c

2+ log. 6ILI Ca`M ZýC

where is a strength efficiency factor that relates the strength of an undirectional short fibre composite to the rule of mixtures prediction.

The factors discussed in this review affecting the strength of a glass reinforced nylon are displayed schematically in Figure 9.

1.5.4 The Toughness of Discontinuous Fibre Composities

Few materials are selected for a structural use on the basis of one property alone, usually a balance of properties of strength, stiffness and toughness are required. Toughness however is even more difficult to predict than stiffness and strength. For many composites the conditions that lead to high stiffness and strength also result in low elongation to break, so that the toughness of a material can vary quite unpredictably24.

Much effort has been devoted to defining parameters which relate applied stress, the size of an existing crack and sample geometry to allow toughness or resistance to crack propagation to be defined in the same way that a modulus can be used to define toughness. One is via an energy approach G,,, the other by a stress intensity factor K,.

Via an Energy Approach

When a body is stressed, energy is stored in the material as strain energy. If a crack extends, some of the energy is released. By equating the energy released to that absorbed in plas- tic deformation and creating new fracture surfaces, it is possible to derive a `strain energy release

-15-

rate', G. , which should be constant at failure. The general solution for calculating G, which is applicable to any loading system is: -

Pi dc G` B da

where Pf is the applied load at failure, B is the thickness, a is the crack length and dC/da is the change in compliance C (1/stiffness), with respect to crack length increase, da.

For many modes of loading with axisymmetric cracks, presuming a linear stress-strain curve where the stored energy is 1f2ac which can often be assumed to be correct for plastics, G, can be calculated as:

xCF; A E

where 2a = crack length, where Q,,, is the failure stress and E the material modulus. (Note that Gi=2a, where a is the "Griffith" surface energy).

Via a Stress Intensity Factor K

By consideration of the detailed stress field at the tip of a sharp crack, it has been shown

that the degree of stress intensification can be more precisely defined by a parameter K- known

as the stress intensity factor. For a crack in a thin plate under tension (where the crack dimen- sions are small compared with overall plate dimensions) K is given by

K na

where a is the applied stress and 2a the crack length. It is postulated that there is a critical value, K, ., at the onset of cracking given by:

"c-aucyim

where a., is the gross failure stress. The value of Kc is referred to as the fracture toughness.

Although the above outline is correct, it is simplistic. Frequently the crack dimensions and

"correction factors", Y, have to be used to account for finite plate effects.

The symbol KI is used to denote opening mode (mode I) fracture in which the crack is open-

ing normally under tensile stress. Mode II refers to shear stresses acting parallel to the direction

"16-

of crack propagation, and mode III refers to shear stresses acting parallel to the crack tip. As nei- ther modes II or III have received significant attention in the polymer literature, these mode of stressing are not considered in this thesis.

In the past before the introduction of instrumented impact testers, assessments of toughness have been based on estimates of work of fracture using Charpy or Izod tests. These measure the amount of energy absorbed from a swinging pendulum striker. The tests however are not easily related to conditions which may be encountered in service.

The value of Gc for a fibrous composite is very often much higher than can be accounted for by adding the contributions of the matrix and the fibre. Much argument has centred on the interactions between these two components responsible for this large increase. Cook and Gor- donu, in their now classic crack blunting mechanism, suggest crack insensitivity may be pro- duced by providing an interface parallel to the fibres which is weak in tension.

Theories perhaps more relevant to short fibre composites include that of Outwater and Mur-

phy26 who argued the energy required to debond a fibre from the matrix is the predominant energy governing the total fracture energy. This theory is supported by McGarry and Mandel27 and Beaumont and Phillips28. Cottrell" obtained a relationship that the fracture energy produced by fibre pull out (U) was related to fibre length by the following expression: -

Ual2 when 1< le Uac j

when I> 1, U=UU when 1=1,

Such a variation is found for discontinuous fibres by Cooper and Kelly3° and Cooper31 using discontinuous flawed fibres and Helfet and Harris32 using chopped wires in a polyester resin.

Kelly presents an analysis33 which suggests the work of fibre pullout is always greater than that of debonding. It seems likely that neither is predominant for all composites but the largest contri-

, 3s.

34buter depends on fibre and matrix type and fibre surface treatment

Rule of mixtures model fora unidirectional composite

____E___

Eý EM

V5 l -V5

. ... "

Figure 1

Theoretical solutions of the isolated fibre

in a matrix

H. L. COX 1952

Fibre

a

Matrix

Considers an elastic fibre completely bonded into an elastic matrix which is subjected to uniform strain along the direction of the fibre axis.

There is no load transferred through the ends of the fibre.

all

J. 0 OUTWATER 1956

40

Ü

Fibre

Thin layer of matrix

Theory Involves a film of negligible thickness which shrinks on to the fibre reinforcement.

This film does not deflect In shear.

Once the initial adhesive bond is broken the resin slides off of the fibre and

the frictional force between resin

and fibre enables further load to be transferred to the fibre as the strain on the composite is Increased.

N_ F DOW 1963

0 Axial load is supplied to a cylindrical matrix containir

fully bonded elastic fibre. No matrix is present at the end of the fibre The solution implies that the initially straight lines remain straight after deformation.

Two and three Dimensional configurations have been analysed

Figure 2q

Theoretical solutions of the isolated fibre in a matrix continued

W_ B_ ROSEN 1964

Fibre

Composite materi SIP Modification of Dows theory.

Fibre surrounded by a material

having average properties of the

f_ _ý

composite. The fibre and average

material only carry tensile stresses and the matrix only carries shear

stresses.

Matrix

A. KELLY and W. R_ TYSON 1965

0

40, Model consists of a elastic fibre in a plastic matrix-The plastic matrix

Cr flows when the shear stress reaches an critical value.

Figure 2b

The definitions of symbols used in The Cox Shear Lag Analysis

### a

Fibre

### .. ý....

Figure 3

x=o Xz

DEPENDENCE OF STIFFNESS ON FIBRE LENGTH

Nylon 66 containing 13 % vol carbon fibres

40 -$- COX

--M- RULE OF MIXTURES

CL 0

0 30

En J

a O 20 7-

w _{J_ }

ui Z

10

a

Figure 4

FIBRE LENGTH (mm)

DEPENDENCE OF STIFFNESS ON FIBRE LENGTH

Nylon 66 containing 8% vol glass fibres

y

CL 0

11 7

J

6 0 m5 W J_

N Z4 W F-

3

0V ki N

ý- COX

-- RULE OF MIXTURES

Figure 5

z o "- un n4

FIBRE LENGTH (mm)

DEPENDENCE OF STIFFNESS ON FIBRE LENGTH

Polypropylene containing 8.5% vol Kevlar fibres

15 -. e-- COX

v 0

En 10 0

w _{J }

Vl 5 Z

w F-

012345

FlBRE LENGTH (mm)

- RULE OF MIXTURES

Figure 6

DEPENDENCE OF STIFFNESS ON FIBRE LENGTH

Nylon 66 containing 12% vol Kevlar fibres

20 e- COX

- RULE OF MIXTURES a 0

0 15

J

a010

m

W J_

z 15

0 "1 hN

Figure 7

FIBRE LENGTH (mm)

a-f..

The variation of tensile stress along a fibre according to Kelly and Tyson

Figure 8

0

bic

### R<Fý I =Rý

Factors influencing the strength of composites

Glass reintorced nylon 66.

S t

r e

n 9

t h

Higher

concentration More

Orientation ý-ý

longer

Bether : fibres

bonding

Shorter

-- obres

0.01 i. 1 1.0 10

Fibre length (mm)

Figure 9

-17- 2.1 Composite Materials

A precise definition of a composite material is difficult to formulate. According to the Encyclopedia of Polymer Science and Technology36 composites can be defined as combinations of materials differing in composition or form on a macroscopic scale and having constituents that retain their identities and do not dissolve or otherwise completely merge into each other. This definition is not strictly accurate as it includes some materials not often considered to be compo- sites. Also some combinations may be thought of as composite structures rather than composite materials, the dividing line is not sharp and differences in opinion do exist. Within this definition examples of composite materials can be identified, from straw filled mud bricks to ceramic whisker filled epoxy used in space shuttles.

Within the last 35 years there has been a rapid growth in the use of all types of plastics.

These materials have found an ever widening use in structural applications, where plastics con- taining reinforcing additives have become well established.

Parrattt and Maxwell37 attempted to list the principal benefits of reinforcement over con- ventional bulk materials.

1. Higher specific strength 2. Higher specific stiffness

3. Enhanced heat deflection temperature 4. Better dimensional stability

5. Better impact and shock resistance 6. Better creep strength

7. Better fatigue strength

8. Control of thermal conductivity and electrical conductivity possible

Thermoplastics containing short fibres were first introduced on to the market with the inten- tion of producing a new range of materials with intermediate properties between the high tonnage commodity plastics and the sophisticated continuous fibre reinforced composites well established

18-

in the aerospace Industry. The increase in stiffness and strength compared with the parent ther- moplastic was modest but sufficient to establish this class of material in lightly stressed applica- tions.

Virtually all common thermoplastics can be reinforced. The widest variety of materials are reinforced with glass fibre. The earliest commercial source for these materials was the Fibrefill process by which production of reinforced polystyrene was started in 195531. Applications included land mines, which required high stiffness and strength but non metallic properties to escape detection devices.

When discussing fibre reinforcement of thermoplastics it is worthwhile to recognise the difference between crystalline and amorphous polymers. The amorphous engineering materials (notably polycarbonate, ABS and polyphenylene oxide) are valued for their low shrinkage and good impact strength, but their fatigue and chemical behaviour can be suspect in common environmental conditions. Crystalline plastics are much more affected by temperature but this deterioration is corrected very positively by reinforcement. Data presented in Table 1 is taken from a publication by Maxwell37 indicates the benefits of reinforcement possible by the incor- poration of 30% glass fibres. The requirements of structural and mechanical components are more likely to be met by crystalline thermoplastics.

During the last few years there has been some significant advances in the development of very high melting point thermoplastics for example, Polyethersulphones (Amorphous). Polyeth- eretherketones (Crystalline) together with a gradual reduction in costs of specialised fibres such as carbon. Materials manufacturers are now combining engineering thermoplastics with more expensive fibres to produce a new range of products. There still is however research required into the fabrication technology necessary to optimise the mechanical properties of these high applica- tion temperature short fibre reinforced thermoplastics.

2.2 Reinforcing Fibres

This survey attempts to review briefly the background of the reinforcing fibres used in this

-19- study and outline some of their salient properties.

2.2.1 Carbon Fibres

Carbon fibres had been known for nearly a century when Thomas Edison first used them as filaments for incandescent lamps. These were produced from the carbonisation of bamboo and rayon. This use for carbon fibre was abandoned after the development of tungsten fibres.

The present activities in the development and use of carbon fibres stems from the work car- ried out in the late 1950's early 1960's in America, Britain and Japan. In America work was ini- tiated on Rayon based carbon fibres and led to Union Carbide's introduction of the Thomel car- bon fibres.

At approximately the same time Shindu38 in Japan and Watt39 and his co-workers in Britain working independently successfully prepared carbon fibres from polyacrylonitrile (P. A. N. ).

These carbon fibres had relatively low strength but high modulus. The mechanical properties of these P. A. N. based carbon fibres were further enhanced by carrying out certain oxidative treat- ments under stress.

The stages in the current production method of P. A. N. based carbon fibre is shown in Figure 10. The P. A. N. fibre is first subjected to oxidisation in air at 200-300°c. During this process the fibre is stretched to obtain carbon fibres of a high quality level. Oxidation will lead to the forma- tion of a ladder polymer consisting of condensed and partly hydrogenated pyridine rings. The subsequent treatment in an inert atmosphere serves to remove hydrogen and nitrogen. Tempera- tures between 1000 and 1300°C produce fibres having high strength (type II) while additional heat treatment at temperatures between 2000 and 3000°C produce graphite fibres having a very high tensile modulus of elasticity (type I). To improve adhesion to the matrix the fibres are sometimes subjected to an oxidative surface treatment and then provided with a finish. The vari- ation of strength and stiffness found with graphitisation temperature is shown in Figure 11.

Figure 12 based on values taken from Hull40 compares the specific properties of the fibres used in this study. From the data it is apparent that the specific modulus of carbon fibre is five